## Bianisotropic Effective

## Parameters of Optical

## Metamagnetics and

## Negative-Index Materials

### An overview of some principles in development of bianisotropic homogenization

### techniques for metamaterials is given in this paper with examples in

### passive and active optical metamaterials.

### By

### A l e x a n d e r V . K i l d i s h e v ,

### Senior Member IEEE

### ,

### J o s h u a D . B o r n e m a n

### ,

### X i n g j i e N i

### ,

### V l a d i m i r M . S h a l a e v ,

### Fellow IEEE

### , a n d V l a d i m i r P . D r a c h e v

ABSTRACT

### |

Approaches to the adequate homogenization of optical metamaterials are becoming more and more complex, primarily due to an increased understanding of the role of asym-metric electrical and magnetic responses, in addition to the nonlocal effects of the surrounding medium, even in the simplest case of plane-wave illumination. The current trend in developing such advanced homogenization descriptions often relies on utilizing bianisotropic models as a base on top of which novel optical characterization techniques can be built. In this paper, we first briefly review general principles for developing a bianisotropic homogenization approach. Second, we present several examples validating and illustrating our approach using single-period passive and active optical metamaterials. We also show that the substrate may have a significant effect on the bianisotropic characteristics of otherwise symmetric passive and active metamaterials.KEYWORDS

### |

Bianisotropic media; homogenization; metamag-netics; metamaterials### I .

### I N T R O D U C T I O N

A new class of nanostructured materials (often called op-tical metamaterials) makes it possible to achieve opop-tical properties that do not exist in nature [1]. Predicting and describing the effective behavior of optical metamaterials in general requires knowledge of their wavevector- and wavelength-dependent dispersion [2]. Upon plane wave excitation though, the effective properties of a thin meta-material layer can be evaluated using a standard ho-mogenization approach [3]–[5], which approximates a nanostructure with a homogeneous layer equivalently producing the same complex transmission and reflection coefficients at normal incidence. However, in actual nano-structured optical metamaterials, due to realistic fabrica-tion tolerances and the necessity for mechanical support with a single- or multilayer substrate, the geometry will inevitably become asymmetric, causing different reflec-tions and even transmissions upon front-side and back-side illumination.

This paper deals with the theoretical fundamentals of bianisotropic homogenization, as it applies to passive and active optical metamaterials (MMs). It reviews the basic structure of 2-D optical metamagnetic and negative-index materials (Section II) and presents the details of the ma-thematical apparatus behind a particular case of bianiso-tropic homogenization upon normal incidence of light (Section III) for a general nonreciprocal material. The paper then examines the spectral dependencies of their retrieved effective parameters (Section V). A special effort Manuscript received June 20, 2010; revised May 29, 2011; accepted June 19, 2011. Date

of publication August 12, 2011; date of current version September 21, 2011. This work was supported in part by the U.S. Army Research Office Multidiciplinary University Research Initiative (ARO-MURI) under Grants 50342-PH-MUR and

W911NF-09-1-0539 and by the U.S. Office of Naval Research (ONR) under Grant N000014-10-1-0942.

A. V. Kildishev,X. Ni,V. M. Shalaev, andV. P. Drachevare with the Birck Nanotechnology Center, School of Electrical and Computer Engineering, Purdue University, West Lafayette, IN 47907 USA (e-mail: a.v.kildishev@ieee.org). J. D. Bornemanwas with the Birck Nanotechnology Center, School of Electrical and Computer Engineering, Purdue University, West Lafayette, IN 47907 USA. He is now with NSWC Crane Division, Crane, IN 47522 USA.

is made to analyze the influence of the substrate on other-wise symmetric structures. Numerical and analytical techniques for validating the proposed approach are addi-tionally discussed in Section IV, where a special case of reciprocal media is considered.

Since the structural asymmetries are not incorporated into a standard homogenization scheme, their effects on the electromagnetic properties cannot be directly em-ployed in a wave dynamics model even at the simplest case of plane wave excitation. Challenges in retrieving the ef-fective properties also arise with when embedding gain materials, as the magnitude of the gain grows and the influence of the asymmetries on active modes becomes increasingly important, just because the standard homoge-nization only accounts for symmetric intrinsic impe-dances, and the parameters it predicts at elevated gain levels could be overestimated.

### I I .

### M E T A M A G N E T I C S A N D

### N E G A T I V E - I N D E X M A T E R I A L S

This section deals with single-period optical MMs, includ-ing optical metamagnetics and negative-index materials. For the time being it suffices to state that the wave equa-tion of such structures allows for 2-D scalar implementa-tion, where the TM case (the single component of the magnetic field is perpendicular to the propagation direc-tion of the incident light and to the periodicity direcdirec-tion) is of prime interest here.

Optical metamagnetics (OMs) are a class of artificially fabricated optical materials (MM) that are designed to produce a strong magnetic response at optical frequencies. OMs can be obtained, for example, using 1-D subwave-length-periodic arrays of nanofabricated silver strip pairs separated by a dielectric spacer as shown in Fig. 1(a). These structures exhibit unusual (artificial) magnetism, not available in nature at the optical range. Studies of OMs have been an important part of MM research [1], [6]–[17] in the area of optical MMs because no negative-index ma-terial is achievable without an artificial magnetic response (due to the necessary condition for obtaining a negative index) [18], [19].

Negative-index metamaterials (NIMs) are yet another class of optical MMs that are designed to produce negative refraction, axis-free imaging, super resolution, and other effects [20]. In the simplest case of an effectively uniform medium, control of the electromagnetic waves is thought to be accomplished through the effective permittivity and permeability "[21], [22]. The effective and "is a result of some averaging of the intrinsic parameters, per-mittivity, and permeability, in electromagnetic MMs. Related to this is the mechanics of wave propagation in hyperbolic MMs or indefinite index media [23]–[27] and more general MMs based on the transformation optics (TO) concept [17], [28], [29]. So called double-negative NIMs are passive MMs with simultaneously negative real parts of and", in contrast with single-negative NIMs where only the real part of"is negative.

Along with a popular fishnet design [1], [30], [31], an alternative structure, shown in Fig. 1(b), could serve the same purpose. Thus, this paper deals with a double-negative NIM arranged as a combination of a 2-D metamagnetic with two continuous metal films [Fig. 1(b)] [7]. Although an optimal design proposed in [28] required previously challenging fabrication of ultra-thin films, this drawback now can be readily alleviated by using a Ge wetting technique resulting in low-loss ultrathin Ag films [32], [33].

### I I I .

### B I A N I S O T R O P I C H O M O G E N I Z A T I O N

A very first method for improving the homogenized MM description is to use bianisotropy (BA) for the material description of the effective slab [34]–[38]. This approach takes into account the nonreciprocal reflection of asym-metric MMs and simultaneously accounts for combined symmetric and asymmetric electric responses, so that some difficulties in the effective characterization of OMs are alleviated.This section presents the fundamentals of the BA ho-mogenization, provided that only normally incident light is used. The homogenization for a realistic case of MMs deposited on a covered substrate are discussed here.

The study done by Chen et al.[36] deals with the in-trinsically asymmetric unit cell structure placed in free space without any super- or substrate. Another asymmetric unit cell structure (in the presence of a uniform substrate and associated nonlocal effects) is rigorously analyzed in related works [35], [39], and [40]. In contrast to those studies: 1) we show that the nonlocal effects of the substrate are quite important even for ideally symmetric unit cell, and cannot be ignored especially in thin samples; 2) we introduce an additional thin adhesion layer into the retrieval of BA parameters; and finally and most impor-tant, 3) we show that the resulting effective BA slab on a substrate can be alternatively described by unidirectional gradients of the complex permittivity~"ðxÞand permeabil-ity~ðxÞ, which are different for the front-side or back-side

Fig. 1.The cross sections (a) of a typical metamagnetic and (b) of an example 2-D negative-index material.

illumination. A less general version of our retrieval technique has been used for the numerical analysis and experimental demonstration of active optical MM with negative index of refraction [41].

A. Effective Parameters of a Bianisotropic Slab

Throughout the paper the monochromatic
time-dependent termse!t _{are omitted and the free-space }
pa-rameters0,k0¼2=0,c0 ¼1=pﬃﬃﬃﬃﬃﬃﬃﬃﬃ"00,z0¼pﬃﬃﬃﬃﬃ0= ﬃﬃﬃﬃﬃ"0

p

, "0, and0, respectively, denote the wavelength, the

wave-number, the velocity of light, the intrinsic impedance, the permittivity, and the permeability.

For the TM case, we define the fieldsE¼^yey,H¼ ^

zhz,D¼^ydy,B¼^zbz; then, using a matrix notation as

f ¼ ey

hz

d¼ dy

bz

(1)

and introducing the curl operator c¼i_{r}@_{x}, and the BA
material matrixm, we combine the Maxwell curl
equa-tions into a matrix form

@d=@t¼k0mf ¼cf (2)
withi_{r}¼ 0 1
1 0
, andm¼ z
1
0 " u
v z0

, where the
ma-terial matrixm, along with relative permittivity"and
rela-tive permeability, includes bianosotropic parametersu;v.
The electric field inside the BA slab (see Fig. 2) can be
written as the forward wave ðe13¼a13ek0n13x_{Þ}_{, and the}
backward wave ðe31¼a31ek0n31x_{Þ}_{, and following the}
formalism of (1), we may now define the field in the slab as

f_{13} ¼ 1
z1
0 z131
a13ek0n13x _{f}
31 ¼
1
z1
0 z311
a31ek0n31x
(3)

where z13;n13 and z31;n31 are the impedance and the refractive index for the forward and backward waves, respectivelyVanother set of BA parameters that should be linked to the terms of matrixm.

First, using (2), we arrive at the dispersion identities

ðmn13irÞ f13¼0 ðmþn31irÞ f31¼0 (4)

where in order to satisfy the Maxwell equations the following identities should initially hold:

z13¼"1ðn13uÞ z31¼"1ðn31þuÞ: (5)

Then, from (4), we arrive at

jmn13irj ¼0 jmþn31irj ¼0: (6)

Thus, solving (6), we have

"¼ ðn13vÞðn13uÞ ¼ ðn31þvÞðn31þuÞ (7)

and we may write

n13¼1 2 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 4"þ ðuvÞ2 q þuþv n31¼1 2 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 4"þ ðuvÞ2 q uv : (8)

We will note an important reduction obtained directly from (8), first by multiplying the solutions, and then by subtracting them

n13n31¼"uv n13n31¼uþv: (9)

Finally, provided thatn136¼n31andz13 6¼z31are given,

the effective parameters ",,u, and vare obtained first from (7), and (9)

"¼ ðn13þn31Þ=ðz13þz31Þ u¼"ðn13z31n31z13Þ=ðn13þn31Þ v¼n13n31u

¼ ðn13n31þuvÞ=": (10)

Fig. 2.Propagation through a bianisotropic slabð0xx0Þ, characterized byn13;z13andn31;z31, the impedance and the refractive index of the forward and backward waves, respectively. The slab is covered by a semi-infinite superstrate layerðx0;n1;z1Þand is deposited on a cover layerðx0GxGxb;n3;z3Þplaced on top of semi-infinite superstrate layerðxbGx;n4;z4Þ. (a) Illumination from the superstrate side. (b) Illumination from the substrate side.

The above defines the sequence of conversion from
parametersz13;n13 andz31;_{n31V}which are available from
experimentVto unknown parametersu,v,, and". The
particular case ofu¼ vmatches [35], [39].

Using the notation of (3), the fields can be defined in the following regions: fields in thesuperstrate layer(region

xG 0) can be expressed asf_{1}ðxÞ ¼z1

0 z

1

1 us1a1, fields in

the BA layer (region 0xx0) can be expressed as

f_{2}ðxÞ ¼z1

0 v2diagðz13;z31Þ

1_{s}

2a2, fields in thecover layer

(region x0 Gxxc) can be expressed as f3ðxÞ ¼

z1

0 z31us3a3, and fields in the substrate layer (region xc Gx) can be expressed asf4ðxÞ ¼z01z41us4a4, where

s1¼diag s1;s11
s1¼ek0n1x _{s}
2¼diagðs13;s31Þ
s13¼ek0n13x s31¼ek0n31x
s_{3}¼diagðs3;s_{3}1Þ s3¼ek0n3x
s4¼diag s4;s41
s4¼ek0n4x
z_{i}¼diagð1;ziÞ; i¼0;1;3;4
and
u¼ 1 1
1 1
v2 ¼
z13 z31
1 1
a1 ¼
a12
a21
a_{2}¼ a13
a31
a_{3}¼ a23
a32
a_{4}¼ a34
a43
:

Using the standard boundary conditions

z_{1}1ua1¼v2diagðz13;z31Þ1s2a2
a_{2}¼ v_{2}diagðz13;z31Þ
1_{s}
2ðx0Þ
1
z_{3}1us_{3}ðx0Þa3 (11)
a_{3}¼ z_{3}1us_{3}ðxcÞ
1
z_{4}1us_{4}ðxcÞa4 (12)
we obtain
tz_{1}1ua_{1}¼t_{3}1z_{4}1u~a_{4} (13)
wheret3¼z31us3ðxcx0Þu1z3,a~4¼s4ðxcÞa4, then
z_{4}t_{3}tz_{1}1 a12þa21
a12a21
¼ ~a34þ~a43
~
a34~a43
(14)

and hence, the transfer matrix is

t¼v2s2ðx0Þv21: (15)

Dividing the field magnitudes in (14) either by the superstrate side incident magnitudea12, or by the substrate side incident magnitude~a43, we arrive at

tz_{1}1 1þr1
1r1
¼t_{3}1z_{4}1 t4
t4
tz_{1}1 t1
t1
¼t_{3}1z_{4}1 r4þ1
r41
(16)

to finally get the transfer matrix connection

t¼t_{3}1z_{4}1wz_{1}
w¼
t4 r4þ1
t4 r41
! _{1}_{þ}_{r}
1 t1
1r1 t1
!1
: (17)

Now, we need to convert (17) into (15) using factorization, thus obtaining z13, z31,s13, and s31 through one to one comparison. To perform such eigendecomposi-tion, we write the transfer matrix as

t¼ t11 t12

t_{21} t_{22}
!

(18)

and after bringing in auxiliary parameters , , 2_{,}

and
¼t_{11}t_{22} 2¼4t_{12}t_{21}
¼t11þt22 ¼
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
2_{þ}_{}2
p
(19)

the factorization of (17) gives the analog of (15), with

v_{2}¼ ðÞ=ð2t21Þ ðÞ=ð2t21Þ

1 1

!

: (20)

Then, the diagonal terms ofs_{2}can be obtained from

s13¼

1

2ðÞ s31¼

1

Finally, the effective parameters of the BA slab are n13 ¼ ðk0x0Þ1cos1 1 2½s13þ1=s13 n31 ¼ ðk0x0Þ1cos1 1 2½s31þ1=s31 (22) z13 ¼ ðÞ=ð2t21Þ; z31¼ ðÞ=ð2t21Þ: (23)

Once the values of n13,n31,z13, and z31 are obtained from the measured complex transmission and reflection coefficients, the effective parameters ", , u, and v are retrieved using (10). An appropriate branch in (22) and (23) should be selected using the conventional restriction [2], [34]–[36] for passive MMs. For the active MMs exa-mined in this paper, maintaining the continuity ofReðnÞ

andImðnÞproduced straightforward retrievals.

B. Numerical Modeling of a Bianisotropic Slab

It is also desirable to model BA samples using, for example, 2-D (scalar) finite element TM solvers. We con-sider a propagatingH-field inside a BA slab ashj ¼h13;j¼

h31;j;E-field is thenej¼z0ðz13h13;jz31h31;jÞ, where indexj denotes either superstrate-side (i.e., front-side f) or substrate-side (i.e., back-side b) illumination, as shown in Fig. 1. To separate the waves within the slab we have to write the identities for the forward (24) and backward (25) wavesðj¼f;bÞ h13;j¼ ðk0n31hj@hj=@xÞ k0ðn13þn31Þ ½ (24) h31;j¼ ðk0n13hjþ@hj=@xÞ k0ðn13þn31Þ ½ : (25)

Then, the magnetic flux densitybj¼b13;jþb31;j and the displacement vectordj¼d13;jþd31;j can be obtained from (2) usingmas dj¼c01 ðz13"þuÞh13;j ðz31"uÞh31;j bj¼0 ðþz13vÞh13;jþ ðz31vÞh31;j : (26)

If we consider a general definition of inhomogeneous
optical material parameters as the ratio between the
mag-netic flux and the magmag-netic field, or between the
displace-ment vector and the electric field, then we may express the
inhomogeneous relative permittivity~_{j}and permeability"~j
for the bianisotropic TM model as

~

_{j}¼bj=ð0hjÞ "~j¼dj=ð"0ejÞ (27)

and as before j denotes either superstrate-side ðfÞ or
subtstrate-side ðbÞ illumination (for the particular cases
considered here, due to the periodic symmetry, the
effec-tive inhomogeneous parameters ~_{j} and "~_{j} change only
along the propagation direction). Equations (27) together
with (24) and (25) are used as auxiliary differential
equa-tions that are solved consistently within a shared FE
computational domain using a commercial FE software

(COMSOLMultiphysics).

This approach is also addressing vital questions on
1) how (and whether it is even possible) to get an effective
description of an MM using the unique distributions of
only two gradient parameters~_{j}ðxÞand~"jðxÞ, and hence,
2) if those distributions could be physically realized to
substitute the entire BA slab. As we show later on, the
intuitively negative answer to 2) also comes from the fact
that even for reciprocal BA media~_{f} 6¼~_{b}and"~_{f} 6¼~"_{b}.

Alternatively, the validation can also be performed analytically. The coefficients of the fields inside the BA slaba13anda31may be obtained by using (11) and (12). The coefficients of the fields in the substrate for the front-side and back-side illumination are expressed as~a4¼ ðt4;0ÞT

and~a4¼ ðr4;1ÞT, respectively. Therefore, the fields inside

the BA slab are known due to (3). Then, the electric dis-placement and the magnetic flux density inside the BA slab can be obtained using (2). Hence, after getting the total field by superimposing the forward and backward waves, the inhomogeneous relative permittivity ~ and"~ perme-ability for the BA slab can be obtained from (27).

This section gives a homogenization approach
perti-nent to the characterization of a general, either reciprocal
or nonreciprocal thin MM sample deposited on a coated
substrate and illuminated with normally incident light.
The sequence of conversion from measured complex
parameters t1;t4 and r1;_{r4V}which are available from
experimentVto unknown effective parametersz13;n13and
z31;n31is given as follows. First, all the elements of matrix

tare obtained from (17); then, those entries (t_{11},t_{12},t_{21},
andt_{22}) are used to get the auxiliary parameters,,2_{,}

and from (19) and retrieve the elements of s2 ¼

diagðs13;s31Þfrom (21). Finally, usings13,s31, andt21, the

auxiliary parameters and , the effective parameters

n13;n31andz13;z31can be obtained from (22) and (23). An alternative set of the effective BA parameters",,u, andv

is retrieved using (10).

In contrast with constant and illumination-side inde-pendent sets of effective parameters fn13;n31;z13;z31g or

f"; ;u;vg, an important notion of the effective
permit-tivity ~"_{j} and permeability ~_{j} is introduced in this section.
Equations (24)–(27), defining"~_{j}and~_{j}(withjbeing either
superstrate-side f or subtstrate-side b illumination) are
obtained using the Sommerfeld splitting. Due to the
nor-mal incidence and the periodic symmetry, the
inhomoge-neous parameters ~_{j} and ~"j change only along the
propagation direction, and as we also show in Section V,
are illumination-side dependent.

### I V .

### B I A N I S O T R O P I C

### R E C I P R O C A L M E D I A

This section covers an important case of reciprocal media followed by the reciprocity-induced simplifications to the general BA homogenization shown in Section III. Here, all discussions and simulations are dealing with reciprocal media, which are of the most interest for the BA charac-terization of thin MM samples in optics.

In reciprocal media the power transmission is inde-pendent of the illumination side, so that the intensity of light transmitted from to the leftT1¼t2

1z4z11 is equal to

the intensity transmitted to the right T4¼t2

4z1z41 (see

Fig. 2); here, the illumination-side impedances are used to
normalize the incident power. As z4z_{1}1¼t4t_{1}1 ¼ jwj,

jz4j ¼z4,jz11j ¼z11,jt3j ¼1, and as from (17), we have
jz_{4}jjt_{3}jjtjjz1

1 j ¼z4z11, we finally arrive at the

require-ment that the matrix t is simplectic, i.e., jtj ¼ ð1=
4Þð2 _{}_{}2_{Þ ¼}_{1. As a result,} _{s}

2 will be a symplectic

matrix as well ðjs_{2}j ¼s13s311Þ. That means that the
propagation constants are identical for both directions

ðn13¼n31Þand do not depend on the illumination side.

Then, the retrieval (22) and (23) for a reciprocal medium
will degenerate into (s13 ¼s31!s, n13¼n31!n, and
u¼ v)
n¼ ðk0x0Þ1cos1 1
2ðsþs
1_{Þ}
(28)
z13 ¼ ðÞ=ð2t_{21}Þ; z31¼ ðÞ=ð2t_{21}Þ (29)
andz13z31¼t12=t21.

In contrast with Section III, dealing with a more gene-ral case, the BA parameters for reciprocal media are given by much simpler formulas

"¼n 2 z13þz31 ¼n 2 z131þz311 u¼nz31z13 z13þz31 (30)

with a more straightforward analogy to a homogeneous slab.

Thus, effective permittivity "is defined as a ratio of effective indexnto averaged effective impedances, effec-tive permittivityis given by the ratio ofnto the averaged admittances, while BA parameteruis given as a product of

nwith a relative difference in effectivez31andz13.

### V .

### E X A M P L E R E T R I E V A L F O R

### R E C I P R O C A L M E D I A

Here we examine the results of the BA homogenization method on several example geometries. Electromagnetic simulations of these geometries were done using a 2-D spatial harmonic analysis (SHA) method [42], [43] for both

front-side and back-front-side illumination, resulting in complex trans-missionðt1;t4Þand reflectionðr1;r4Þcoefficients. Equations (28), (29), and (30) are then used to determine the effective BA parameters of the MM. In order to validate these results, we then obtain the complex transmission and reflection coefficients of a homogeneous bianisotropic slab with a permittivity and permeability as defined in (27), using FE model described above. As we will show, the coefficients

t1;t4 and r1;r4 obtained from the homogenized BA slab

match those of structured MM, successfully validating the retrieved effective parameters.

First, we examine a simple metamagnetic grating, as
shown in Fig. 1(a). The upper and lower dielectric layers
and the indium tin oxide (ITO) layer are usually present
due to fabrication requirements, and are not necessary to
the fundamental performance of the metamagnetic,
therefore we have removed these layers_{1} ¼ITO¼0 in
order to examine the core three-layer metamagnetic. The
r e m a i n i n g g e o m e t r i c d i m e n s i o n s a r e

fp;w; Ag; sg ¼ f250;120;30;40g[nm]. The SHA simu-lation results are given as the wavelength-dependent phasor diagrams of complex r;t coefficients in Fig. 3(a) and (b), for front-side and back-side illumination, respec-tively. As expected for a reciprocal medium, the substrate-normalized values of t coefficients shown as black solid lines in Fig. 3(a) and (b) are indeed identical

ðt4z1

4 ¼t4n4¼t1Þ, while the spectral phasor diagrams

for complex reflection coefficients (solid red lines) are different. To setup a numerical validation test, the retrieved effective BA parameters are then used in

h13;j¼
1
2 hjðk0nÞ
1_{@}
hj=@x
h31;j¼
1
2 hjþðk0nÞ
1_{@}
hj=@x
ej¼z0ðz13h13;jz31h31;jÞ (31)

Fig. 3.Spectral phasor diagrams for a metamagnetic sample: (a) front-side and (b) back-side illumination substrate-normalized complex transmission coefficients and complex reflection coefficients from a nanostructured metamagnetic (SHA, solid lines) compared to those from the homogenized slab (FEM, circles).

and in simpler equivalents of (26) for reciprocal media dj ¼c01 ðz13"þuÞh13;j ðz31"uÞh31;j bj ¼0 ðz13uÞh13;jþ ðþz31uÞh31;j : (32)

First, (32) is used as auxiliary differential equations (ADE)
in the finite element method (FEM) domain, so that the
local, spatially dependent material parameters inside the
effective BA slab are defined by (27). Once the equations
for ~_{j} and "~j are set, the scalar wave equation for the
transverse magnetic field is then solved self-consistently.
The matchingr;tFEM results for the homogenized slab,
equivalent to a given metamagnetic, are shown as red and
black circles in Fig. 3(a) and (b).

Further insight into the performance of the bianiso-tropic MM may be obtained by examining the relative permittivity ð~"Þ and permeability ð~Þ (27), within the effective slab. Fig. 4 shows"~and~as a function of position in the slab for both front-side and back-side illumination, both with and without the glass substrate.

We also studied the effective parameters of a 2-D NIM [7], as shown in Fig. 1(b). Again, for simplicity, we have removed the ITO layer from the simulationsITO¼0. We used a previously optimized geometry of fp;w; 1; Ag;

Sg ¼ f324;168;20;46;68g[nm]. Spectra andr;t coeffi-cients from SHA are shown in Fig. 5(a), (e), and (f), and the retrieved effective optical parameters are shown in Fig. 5(b)–(d). Again we see that the effective homogenized

slab, also Fig. 5(e) and (f), matches the SHA results of the structured geometry.

We also analyze the relative permittivity ð~"Þand per-meabilityð~Þwithin the 2-D NIM equivalent slab, shown in Fig. 6, which again shows that the presence of the sub-strate induces an asymmetric optical response within the effective medium. Figs. 4(b) and (d) and 6(b) and (d) confirm that for any center-symmetric unit cell arranged of reciprocal elemental materials, not only the optical re-sponse is reciprocal, but it is also nonbianisotropic

ðu;v0Þ, and therefore"~¼",~¼.

The high optical loss (large imaginary refractive index) in these materials warrants the use of a gain medium to enhance the transmission of the sample, and has been discussed at length elsewhere [10]. Therefore, we have also analyzed a 2-D NIM structure, Fig. 1(b), where the dielectrics (alumina and silica) have both been replaced with a simple gain medium.

The permittivity of the simple gain medium is defined using a Cauchy model to simulate the dielectric host (set equivalent to alumina), and uses a negative Lorentz

Fig. 4.Relative optical properties as a function of position for a metamagnetic grating equivalent slab on a glass substrate: (a)"~and (c)~and in air: (b)"~and (d)~. Illumination is at 700 nm from front side (black) and back side (red) (solid: real; dashed: imaginary).

Fig. 5.2-D NIM. (a) TM spectra (solid lines: front-side illumination; dashed: backside), (b) retrieved index of refraction½n[for (b)–(f), solid: real part, dashed: imaginary part], (c) retrieved permittivity½" and permeability½, (d) retrieved bianisotropy½u;v, (e) front-side and (f) back-side illumination complex reflection (r: red) and transmission (t: black) coefficients from metamagnetic (SHA: solid lines) compared to those from the homogenized BA slab (FEM: circles) (red: real part; black: imaginary part).

oscillator (resulting in a negative imaginary n), with an amplitude such that the peak gain is 1000 cm1centered at 780 nm with a width of 100 nm, to simulate the effect of a stimulated emission transition in an embedded dye. This results in a static frequency-domain model for gain, which will of course not represent many transient and intensity-dependent effects, but which is sufficient to represent the effect of a negative imaginary permittivity, with a realistic amplitude and spectral dependence, on the effective medium parameters.

Again, spectra andr;tcoefficients from SHA are shown in Fig. 7(a), (e), and (f), compared to the BA slab Fig. 7(e) and (f), and the retrieved effective optical parameters are shown in Fig. 7(b)–(d). Although the resonances are red-shifted, due to replacing silican¼1:5 with an alumina-like gain materialReðnÞ ﬃ1:62 and narrowed slightly from the dielectric case, we see that the retrieved imaginary refractive index is lower near the wavelength with peak negative refractive index. With no gain, ImðnÞ ¼0:25 at 775 nm, whereas with gain,ImðnÞ ¼0:06 at 810 nm.

### V I .

### S U M M A R Y A N D F U T U R E W O R K

In this paper, we presented an approach to the BA homogenization of optical MMs (including deposited on a covered substrate) and discussed several techniques for validating the retrieved effective parameters of these nanostructures. The theoretical fundamentals of BA homo-genization are developed using the transfer matrix for-malism applied to passive and active optical MMs. First, we use (5), (8), and (10) to develop the sequence ofcon-version from parametersz13;n13andz31;_{n31V}which could

be obtained from experimentVto unknown BA

parame-tersu,v,, and". Then, we compare the transfer matrix with unknown parameters z13;n13 andz31;n31 defined in (15) with the same transfer matrix that could be obtained from the experimental data in (17). The comparison re-sulted in formulas (22) and (23), connectingz13,n13,z31,

n31, with complex transmission ðt4;t1Þ and reflection

ðr1;r4Þcoefficients available from optical characterization

of a given MM sample. That concludes the development of the homogenization approach.

Then, we focus our theoretical development and nu-merical validation solely at the practical case of reciprocal media for which easier analysis is possible. The initial re-ciprocity conditionT1¼T4is satisfied only ifu¼ v, and the propagation constants do not depend on the illumina-tion side, i.e.,s13¼s31!sandn13¼n31!nand simpler (28), (29), and (30) could be used to determine the BA effective parameters of the MM.

This approach was applied to a simple metamagnetic grating and a 2-D NIM. Coefficients t4;t1;r1;r4 were

Fig. 6.Relative optical properties as a function of position for a 2-D NIM equivalent slab on a glass substrate: (a)"~and (b)~and in air: (c)~"and (d)~. Illumination is at 700 nm from front side (black) and back side (red) (solid: real; dashed: imaginary).

Fig. 7.2-D NIM with gain. (a) TM spectra (solid lines: front-side illumination; dashed: backside), (b) retrieved index of refraction½n [for (b)–(f), solid: real part, dashed: imaginary part], (c) retrieved permittivity½"and permeability½, (d) retrieved bianisotropy½u;v, (e) front-side and (f) back-side illumination complex reflection (r: red) and transmission (t: black) coefficients from metamagnetic (SHA: solid lines) compared to those from the homogenized slab (FEM: circles) (red: real; black: imaginary).

obtained from SHA simulations, and the retrieved optical parameters were presented here. This retrieval approach is shown to reproduce the expected electrical and magnetic resonances, in addition to significant BA. Further, FEM simulations using the effective parameters in a homoge-neousBslab[accurately reproduce the complex coefficients of the metal-dielectric MM. These homogeneous FEM simulations are also analyzed to show the distribution of the relative field-ratio parameters~";. This result shows that~ the substrate induced asymmetry (front-side versus back-side illumination) of the field within the slab results in asymmetric values for ~";, as opposed to a symmetric~ geometry with no substrate, which has constant~";~values. Indeed the presence of the substrate is seen to have a significant effect on the retrieved values, and therefore on

the performance and BA of the MM. In essence, the re-trieved effective parameters are certainly nonlocal, embed-ding the influence of substrate–superstrate environment. We would conclude that retrieval and discussion of MM bianisotropic optical parameters cannot be separated from substrate–superstrate media and incidence direction.

A more advanced BA-based characterization method will be used as an advantageous tool for the studies of the effective angular-dependent models of MMs.h

### A c k n o w l e d g m e n t

The authors would like to thank the reviewers for several vital suggestions. A. V. Kildishev would also like to thank N. Engheta for valuable discussions.

R E F E R E N C E S

[1] U. K. Chettiar, S. Xiao, A. V. Kildishev, W. Cai, H. K. Yuan, V. P. Drachey, and V. M. Shalaev,BOptical metamagnetism and negative-index metamaterials,[MRS Bull., vol. 33, pp. 921–926, Oct. 2008. [2] S. G. Rautian,BReflection and refraction

at the boundary of a medium with negative group velocity,[Physics-Uspekhi, vol. 51, pp. 981–988, Oct. 2008.

[3] D. R. Smith, S. Schultz, P. Markos, and C. M. Soukoulis,BDetermination of effective permittivity and permeability of metamaterials from reflection and transmission coefficients,[Phys. Rev. B, vol. 65, May 15, 2002, 195104. [4] W. B. Weir,BAutomatic measurement of

complex dielectric-constant and permeability at microwave-frequencies,[Proc. IEEE, vol. 62, no. 1, pp. 33–36, Jan. 1974. [5] BComments onFAutomatic measurement of

complex dielectric-constant and permeability at microwave-frequencies_,[Proc. IEEE, vol. 63, no. 1, pp. 203–205, Jan. 1975. [6] W. S. Cai, U. K. Chettiar, H. K. Yuan,

V. C. de Silva, A. V. Kildishev, V. P. Drachev, and V. M. Shalaev,BMetamagnetics with rainbow colors,[Opt. Exp., vol. 15, pp. 3333–3341, Mar. 2007.

[7] U. K. Chettiar, A. V. Kildishev, T. A. Klar, and V. M. Shalaev,BNegative index metamaterial combining magnetic resonators with metal films,[Opt. Exp., vol. 14, pp. 7872–7877, Aug. 21, 2006.

[8] C. Enkrich, M. Wegener, S. Linden, S. Burger, L. Zschiedrich, F. Schmidt, J. F. Zhou, T. Koschny, and C. M. Soukoulis,BMagnetic metamaterials at telecommunication and visible frequencies,[Phys. Rev. Lett., vol. 95, 2005, 203901.

[9] A. V. Kildishev, W. S. Cai, U. K. Chettiar, H. K. Yuan, A. K. Sarychev, V. P. Drachev, and V. M. Shalaev,BNegative refractive index in optics of metal-dielectric composites,[

J. Opt. Soc. Amer. BVOpt. Phys., vol. 23, pp. 423–433, Mar. 2006.

[10] T. A. Klar, A. V. Kildishev, V. P. Drachev, and V. M. Shalaev,BNegative-index metamaterials: Going optical,[IEEE J. Sel. Topics Quantum Electron., vol. 12, no. 6, pt. 1, pp. 1106–1115, Nov./Dec. 2006.

[11] S. Linden, C. Enkrich, M. Wegener, J. F. Zhou, T. Koschny, and C. M. Soukoulis,

BMagnetic response of metamaterials at 100 terahertz,[Science, vol. 306, pp. 1351–1353, Nov. 19, 2004.

[12] G. Shvets and Y. A. Urzhumov,

BNegative index meta-materials based on two-dimensional metallic structures,[

J. Opt. AVPure Appl. Opt., vol. 8, pp. S122–S130, Apr. 2006.

[13] S. M. Xiao, U. K. Chettiar, A. V. Kildishev, V. Drachev, I. C. Khoo, and V. M. Shalaev,

BTunable magnetic response of metamaterials,[Appl. Phys. Lett., vol. 95, Jul. 20, 2009, 033115.

[14] H.-K. Yuan, U. K. Chettiar, W. Cai, A. V. Kildishev, A. Boltasseva, V. P. Drachev, and V. M. Shalaev,BA negative permeability material at red light,[Opt. Exp., vol. 15, pp. 1076–1083, 2007.

[15] S. Zhang, W. J. Fan, B. K. Minhas, A. Frauenglass, K. J. Malloy, and S. R. J. Brueck,BMidinfrared resonant magnetic nanostructures exhibiting a negative permeability,[Phys. Rev. Lett., vol. 94, Jan. 28, 2005, 037402. [16] V. A. Podolskiy, A. K. Sarychev,

E. E. Narimanov, and V. M. Shalaev,

BResonant light interaction with plasmonic nanowire systems,[J. Opt. AVPure Appl. Opt., vol. 7, pp. S32–S37, Feb. 2005. [17] A. V. Kildishev and V. M. Shalaev,

BEngineering space for light via transformation optics,[Opt. Lett., vol. 33, pp. 43–45, Jan. 1, 2008. [18] R. A. Depine and A. Lakhtakia,

BA new condition to identify isotropic dielectiric-magnetic materials displaying negative phase velocity,[Microw. Opt. Technol. Lett., vol. 41, pp. 315–316, May 20, 2004.

[19] R. W. Ziolkowski and E. Heyman,

BWave propagation in media having negative permittivity and permeability,[

Phys. Rev. E, vol. 64, Nov. 2001, 056625. [20] V. M. Shalaev,BOptical negative-index

metamaterials,[Nature Photon., vol. 1, pp. 41–48, Jan. 2007.

[21] J. B. Pendry,BNegative refraction makes a perfect lens,[Phys. Rev. Lett., vol. 85, p. 3966, 2000.

[22] V. G. Veselago,BElectrodynamics of substances with simultaneously negative values of Sigma and Mu,[Soviet Physics Uspekhi-USSR, vol. 10, p. 509, 1968. [23] A. J. Hoffman, L. Alekseyev, S. S. Howard,

K. J. Franz, D. Wasserman, V. A. Podolskiy, E. E. Narimanov, D. L. Sivco, and C. Gmachl,

BNegative refraction in semiconductor metamaterials,[Nature Mater., vol. 6, pp. 946–950, Dec. 2007.

[24] D. R. Smith and D. Schurig,BElectromagnetic wave propagation in media with indefinite permittivity and permeability tensors,[Phys. Rev. Lett., vol. 90, Feb. 21, 2003, 077405. [25] D. R. Smith, D. Schurig, J. J. Mock,

P. Kolinko, and P. Rye,BPartial focusing of radiation by a slab of indefinite media,[

Appl. Phys. Lett., vol. 84, pp. 2244–2246, Mar. 29, 2004.

[26] R. Wangberg, J. Elser, E. E. Narimanov, and V. A. Podolskiy,BNonmagnetic nanocomposites for optical and infrared negative-refractive-index media,[J. Opt. Soc. Amer. BVOpt. Phys., vol. 23, pp. 498–505, Mar. 2006.

[27] J. Yao, Z. W. Liu, Y. M. Liu, Y. Wang, C. Sun, G. Bartal, A. M. Stacy, and X. Zhang,

BOptical negative refraction in bulk metamaterials of nanowires,[Science, vol. 321, pp. 930–930, Aug. 15, 2008. [28] J. B. Pendry, D. Schurig, and D. R. Smith,

BControlling electromagnetic fields,[

Science, vol. 312, pp. 1780–1782, Jun. 23, 2006.

[29] A. V. Kildishev, W. Cai, U. K. Chettiar, and V. M. Shalaev,BTransformation optics: Approaching broadband electromagnetic cloaking,[New J. Phys., vol. 10, Nov. 27, 2008, 115029.

[30] S. A. Zhang, W. J. Fan, N. C. Panoiu, K. J. Malloy, R. M. Osgood, and

S. R. J. Brueck,BOptical negative-index bulk metamaterials consisting of 2D perforated metal-dielectric stacks,[Opt. Exp., vol. 14, pp. 6778–6787, Jul. 24, 2006.

[31] C. M. Soukoulis, S. Linden, and M. Wegener,

BNegative refractive index at optical wavelengths,[Science, vol. 315, pp. 47–49, Jan. 5, 2007.

[32] W. Q. Chen, M. D. Thoreson, S. Ishii, A. V. Kildishev, and V. M. Shalaev,

BUltra-thin ultra-smooth and low-loss silver films on a germanium wetting layer,[Opt. Exp., vol. 18, pp. 5124–5134, Mar. 1, 2010.

[33] V. J. Logeeswaran, N. P. Kobayashi, M. S. Islam, W. Wu, P. Chaturvedi, N. X. Fang, S. Y. Wang, and R. S. Williams,

BUltrasmooth silver thin films deposited with a germanium nucleation layer,[Nano Lett., vol. 9, pp. 178–182, 2008.

[34] R. Marques, F. Medina, and

R. Rafii-El-Idrissi,BRole of bianisotropy in negative permeability and left-handed metamaterials,[Phys. Rev. B, vol. 65, Apr. 1, 2002, 144440.

[35] C. E. Kriegler, M. S. Rill, S. Linden, and M. Wegener,BBianisotropic photonic metamaterials,[IEEE J. Sel. Topics Quantum Electron., vol. 16, no. 2, pp. 367–375, Mar.–Apr. 2010.

[36] X. Chen, B. I. Wu, J. A. Kong, and T. M. Grzegorczyk,BRetrieval of the effective constitutive parameters of bianisotropic metamaterials,[Phys. Rev. E, vol. 71, Apr. 2005, 046610.

[37] X. D. Chen, B. I. Wu, J. A. Kong, and T. M. Grzegorczyk,BErratum: Retrieval of the effective constitutive parameters of bianisotropic metamaterials (vol 71, pg 046610, 2005),[Phys. Rev. E, vol. 73, Jan. 2006, 019905.

[38] Z. Ku, K. M. Dani, P. C. Upadhya, and S. R. Brueck,BBianisotropic negative-index metamaterial embedded in a symmetric medium,[J. Opt. Soc. Amer. B, vol. 26, pp. B34–B38, 2009.

[39] M. S. Rill, C. Plet, M. Thiel, I. Staude, G. Von Freymann, S. Linden, and M. Wegener,BPhotonic metamaterials by direct laser writing and silver chemical vapour deposition,[Nature Mater., vol. 7, pp. 543–546, Jul. 2008.

[40] D. A. Powell and Y. S. Kivshar,

BSubstrate-induced bianisotropy in metamaterials,[Appl. Phys. Lett., vol. 97, 2010, 091106.

[41] S. M. Xiao, V. P. Drachev, A. V. Kildishev, X. J. Ni, U. K. Chettiar, H. K. Yuan, and

V. M. Shalaev,BLoss-free and active optical negative-index metamaterials,[Nature, vol. 466, p. 735-U6, Aug. 5, 2010. [42] A. V. Kildishev and U. K. Chettiar,BCascading

optical negative index metamaterials,[

Appl. Comput. Electromagn. Soc. J., vol. 22, pp. 172–183, Mar. 2007.

[43] X. Ni, Z. Liu, F. Gu, M. G. Pacheco, J. D. Borneman, and A. V. Kildishev,

BPhotonicsSHA-2D: Modeling of single-period multilayer optical gratings and metamaterials,[2009, DOI: 10254/ nanohub-r6977.9.

A B O U T T H E A U T H O R S

Alexander V. Kildishev(Senior Member, IEEE) received the M.S. degree in electrical engineering (honors) from the Kharkov State Polytechnical University (KSPU), Ukraine, and the Ph.D. degree in electrical engineering from KSPU in 1996.

He is a Principal Research Scientist at the Birck Nanotechnology Center, School of Electrical and Computer Engineering, Purdue University, West Lafayette, IN. He leads the development of simu-lation methods and software tools for applied

electromagnetics and multiphysics simulations. Before joining Purdue University, he was working as the Head of Laboratory at the Magnetism Division of the National Academy of Sciences in the Ukraine. Currently, his research interests are in the modeling of nanophotonics devices, optical metamaterials, and transformation optics. His publications include four book chapters, four patents, more than 80 articles in peer-reviewed journals, with more than 2000 citations, and more than 30 invited seminar and conference talks.

Dr. Kildishev is a member of the Optical Society of America (OSA), the International Society for Optics and Photonics (SPIE), the Society for Industrial and Applied Mathematics (SIAM), and the Applied Computa-tional Electromagnetics Society (ACES).

Joshua D. Bornemanreceived the M.S. degree in physics and the Ph.D. degree in electrical and computer engineering (working with Prof. V. M. Shalaev’s group) from Purdue University, West Lafayette, IN, in 2004 and 2010, respectively.

He is currently an Engineer for the Navy at NSWC Crane Division, Crane, IN, working on electro-optic science and technology projects. His interests include characterization and simula-tion of metamaterials and nonlinear optics. He has

also worked as a Mathematics Instructor at Purdue University, and as a Technical Intern for Intel Corporation.

Dr. Borneman has been a member of the Optical Society of America (OSA) since 2004.

Xingjie Nireceived the B.S. degree in engineering physics and the M.S. degree in automation from Tsinghua University, Beijing, China, in 2005 and 2007, respectively. He is currently working as a Research Assistant towards the Ph.D. degree in electrical and computer engineering in Prof. V. M. Shalaev’s group at the Birck Nanotechnology Center, School of Electrical and Computer Engi-neering, Purdue University, West Lafayette, IN. He is also working towards the M.S. degree in

computer science under the supervision of Prof. A. Sameh at Purdue University.

His current research interests include modeling and characterization of metamatertials, transformation optics devices, and computational electromagnetics.

Mr. Ni is a member of the Optical Society of America (OSA). Vladimir (Vlad) M. Shalaev (Fellow, IEEE)

re-ceived the M.S. degree in physics (with highest distinction) and the Ph.D. degree in physics and mathematics from Krasnoyarsk State University, Russia, in 1979 and 1983, respectively.

He is the Robert and Anne Burnett Professor of Electrical and Computer Engineering and Professor of Biomedical Engineering at Purdue University, West Lafayette, IN, and specializes in nanopho-tonics, plasmonics, and optical metamaterials. He

authored three books, 21 book chapters, and over 300 research publica-tions, in total.

Prof. Shalaev received several awards for his research in the field of nanophotonics and metamaterials, including the Max Born Award of the Optical Society of America (OSA) for his pioneering contributions to the field of optical metamaterials and the Willis E. Lamb Award for Laser Science and Quantum Optics. He is a Fellow of the American Physical Society (APS), the International Society for Optics and Photonics (SPIE), and the Optical Society of America (OSA).

Vladimir P. Drachevgraduated from Novosibirsk State University, Russia and received the Ph.D. degree in experimental physics from the Institute of Semiconductor Physics and the Institute of Automation and Electrometry, Russian Academy of Sciences (RAS), Moscow, Russia, in 1995.

He has been a Senior Research Scientist with the Birck Nanotechnology Center and School of Electrical and Computer Engineering, Purdue University, West Lafayette, IN, since 2002. In

1999–2001, he worked as a Visiting Scientist at New Mexico State University. His current research interests include optics and nonlinear optics, nonlinear spectroscopy of nanomaterials, spectroscopy of metal-molecule complexes, biosensing, nano-optics, nanofabrication, plasmo-nics, and metamaterials.

Dr. Drachev has been granted several awards from the International Science Foundation, and the Ostrovskii award (1997) from Ioffe Institute of Russian Academy of Sciences (RAS), St. Petersburg, Russia.